Powder Manufacturing & Quality Control
This section describes the manufacturing and quality control process for powder coating materials. The state of the art technology used for producing industrial powder coatings consists of several distinct stages, namely:
- Weighing, premixing and size reduction of raw materials
- Extrusion of pre-mix, cooling and crushing of the extrudate into chips
- Micronising the chips into the final powder
- Post mixing, packaging and storage.
At each stage of the production process the quality must be checked because once the powder coating material has been produced, it cannot be changed or adjusted in any significant way. The formulation and the manufacturing conditions are therefore critical. Reworking of an ‘out of specification’ product is difficult and costly. (See Figure 1 for a simplified flow sheet of the powder coating material production process).
Weighing, premixing and size reduction of raw materials
Raw materials typically consist of resin, curing agents, pigments, extenders and additives such as flow and degassing aids. Each raw material must pass their individually pre-set quality controls. This is accomplished by auditing the certificate of analysis of the incoming raw material.
Each component is then weighed with the necessary degree of accuracy (which may be to the nearest ten-thousands of a gram). All pre-weighed components are placed in a mixing container according to the formulation. The container is then attached to the mixing drive and the raw materials are thoroughly mixed by the specially designed premixer cutting blades for a pre-set period of time. The raw materials can also be reduced in size to improve the melt mixing later in the process.
A final sample of the raw material pre-mix is checked for conformity and processed through
a small laboratory extruder or the production extruder and grinder. The resulting powder is then applied onto a test panel, cured in the oven and subjected to various tests:
- Color and gloss
- Mechanical performance such as impact testing and solvent resistance.
- Gel time and HPMF
If adjustments are required both the mixing process and quality control procedures are repeated until the powder achieves the specification. This is done for every mix.
No further modification to the powder can be made after this stage in production. If all the quality control measures are met, then the material is moved to the next step extrusion.
Extrusion of the premix
The mix is fed into the dosing system of the extruder. The extruder barrel is maintained at a predetermined temperature (between 70 & 120ºC, depending on the product type). The barrel temperature is set so that the resin is only just liquefied and its contents are mixed using the screw in the barrel. Consequently, the individual ingredients are dispersed and wetted by the resin, which produces a homogeneous composite. The feed rate of the dosing equipment and the speed of the extruder screw are balanced to ensure that the screw is kept loaded within the extruder barrel. The conditions of high shear and intimate mixing are maintained within the extruder by precise adjustments of these three parameters.
The molten mass produced in the extruder barrel is forced to cool down via a cooling-transporting device. The solidified material is then broken up and reduced in size through a crusher into workable chips of 5 to 10mm in size.
At this stage in the process the product quality is tested using a sample of the chips. The laboratory grinds the chips to a powder and prepares a test panel using the material. The intermediate product is then checked for quality against the following criteria:
- Color and gloss
- Impact resistance and solvent resistance
- Gel time and hot plate melt flow
Too high a temperature in the extruder barrel will not only result in a low melt viscosity, low shear forces and poor pigment dispersion, but will also in turn produce a low gloss coating. The resin and hardener in the premix may also start to react in the extruder, which will also have a detrimental effect on the product performance.
It is not possible to make changes to the formulation at this stage in the production process. It is also easier to handle the extruded chip as a re-work raw material if manufactured ‘out of specification’ than once the powder has been micronized.
Micronizing of the chip into the final powder
The chips are ground to the required particle size in a grinding mill. The chips are fed onto an enclosed grinding wheel with stainless steel pins, which breaks the chips down creating a powder. The powder is carried through a classifier into a cyclone collection system via a regulated air flow.
In order to achieve the optimal particle size distribution (psd) further treatment may be needed which can consist of cycloning, classifying, filtering or sieving.
In modern plants the rejected oversize from the sieving operation is automatically fed back into the feed stream of the micronizing mill. The typical particle size range for electrostatic application methods should be within 10 to 100 microns. Deviation from this particle size distribution can result in poor performance and appearance of the powder.
The final powder coating is as rigorously quality control tested to ensure it meets the specification of the customer or market. As the particle size distribution is a critical factor in the successful use of the powder the particles are analysed for their precise particle size distribution.
Post mixing, packaging and storage
In order to meet the customer specification or special conditions of use additives may have to be mixed through the final product. Powder packaging is provided in:
- carton boxes – up to 50 lbs
The powder can be safely stored if kept in its unopened packaging in a dry, cool place (75ºF) for up to 12 months. Higher temperatures and longer storage periods will result in absorption of moisture. Storage conditions can vary for some powders so the product data sheet should be referred to at all times.
It is advisable to check the powder after 6 months of storage to ensure no quality problems have occurred.
Modern powder coating materials from Alpha Coating Technologies can achieve the same quality standards for appearance, chemical and mechanical resistance for future manufacturing. Once a product has completed the development stage and its formulation and manufacturing procedures have been approved, it will be available for manufacturing again at any time in the future.
End of quality control document.
Created by: Jeno Muthiah
Date: Nov 8, 2011